Rutger C. Wijburg, Gertjan J. Hemink, Student Member, IEEE, Jan Middelhoek, Hans Wallinga, ... of programming cycles of such device for E'PROM applica-.
IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 38, NO. 1, JANUARY 1991
Novel Buried Injector Structure for EPROM Applications
Rutger C. Wijburg, Gertjan J. Hemink, Student Member, IEEE, Jan Middelhoek, Hans Wallinga, and Ton J. Mouthaan, Member, IEEE
Abstract-A buried injector is proposed as a source of electrons for substrate hot electron injection. To enhance the compatibility with VLSI processing, the buried injector is formed by the local overlap of the n-well and p-well of a retrograde twin-well CMOS process. The injector is activated by means of punchthrough. This mechanism allows the realization of a selective injector without increasing the latchup susceptibility. The p-well profile controls the punchthrough voltage. The high injection probability and efficient electron supply mechanism lead to oxide current densities up to 1.0 A . Em-’. Programming times of 10 ps have been measured on nonoptimized cells. The realization of a structure for 5-V-only digital and analog applications is viable. A model of the structure for implementation in a circuit simulator, such as SPICE, is presented.
N increasing demand exists for high-performance EPROM’s and E2PROM’s in digital applications. In the near future, magnetic media may be replaced by E’PROM’S [ 11. However, also in analog and analog-digital applications adjustable components are required. EPROM’s can be used in analog CMOS circuits. In this way, it is possible to cancel offsets in differential amplifiers . E’PROM’s may also find application in adaptive filters or in neural networks , . In this paper we will describe a new structure for an EPROM device, which is realized by high-energy ion implantation and may be used in various EPROM applications. The paper focuses on the working principle of the realized structure and its modeling. Furthermore, programming characteristics of nonoptimized memory cells are given, in order to demonstrate its high speed potential. In a following paper, the performance of optimized cells and method of cell selection in a memory matrix will be discussed based on the evaluation of a 16K flash-E’PROM . Conventional EPROM’s widely use the method of Channel Hot Electron (CHE) injection for programming. Electrons that become hot in the pinchoff region have a small probability of being injected into the gate oxide and flowing to the floating gate. The electrons should gain sufficient kinetic energy in the electrical field parallel to the Si-Si02 interface and then they have to be redirected towards the Si-Si02 interface . The influence of the drain and gate voltage on the number of hot carriers and the height of the Si-Si02 potential barrier lead to conflicting demands , . Therefore, high drain and gate voltages are often used as a compromise in practical programManuscript received January 2, 1990; revised June 5, 1990. This work was supported by the Foundation for Fundamental Research on Matter (FOM) and the Netherlands Technology Foundation (STW). The review of this paper was arranged by Associate Editor B. Ricco. R. C. Wijburg, G. J. Hamink, H. Wallinga, and T. J. Mouthaan are with the Faculty of Electrical Engineering, University of Twente, P.O. Box 217, 7500 AE Enschede, The Netherlands. J. Middelhoek, deceased, was with the Faculty of Electrical Engineering, University of Twente, 7500 AE Enschede, The Netherlands. IEEE Log Number 9040178.
ming. As a result, drain-side CHE injection EPROM’s have a low injection probability. They generally do not allow 5-V-only operation, although for some drain-side CHE injection EPROM’s with submicrometer channel length the programming drain voltage can be reduced to 5 V . The source-side CHE injection technique can be used, in order to overcome these disadvantages . However, as in the case of a drain-side CHE injection EPROM, the injection of hot electrons is limited to a very small region. As the charge injection is the driving mechanism for oxide breakdown [lo], the lifetime and the number of programming cycles of such device for E’PROM applications are restricted. An alternative method to the CHE injection is the Substrate Hot Electron (SHE) injection, which is shown in Fig. 1. The source of electrons is the substrate. The SHE injection has several advantages. Electrons that are accelerated in the depletion layer underneath the gate and become hot are directed towards the Si-Si02 interface. The injection probability can be increased by raising the gate voltage, which lowers the Si-Si02 potential barrier -. In contrast to the conventional CHE injection, this can be done without decreasing the number of hot electrons. The SHE injection technique can be applied in a 5-V-only EPROM, because the only higher voltage needed on chip is connected to the gate terminal of high impedance and can be generated on chip by charge pumping techniques . The injection of electrons can take place over nearly the whole active gate area. In the case of equal injection current the SHE injection offers a lower oxide current density than the CHE injection. Because the oxide is stressed less locally, a higher reliability of the SHE injection EPROM may be expected compared to the CHE injection EPROM. In addition, both normal CMOS and EPROM devices can use the same advanced source and drain structures in order to suppress unwanted shortchannel effects (151. The major problem associated with the conventional SHE injection is the method for generation of electrons in the substrate. Photogeneration and avalanche multiplication have been used. Verwey et al. [ 161 employed a forward-biased n-type substrate with a p-type epilayer. Eitan et al.  used a forwardbiased p-n junction, which was situated closely to the EPROM device. Such a forward-biased p-n junction has low injection efficiency, because only a small part of the injected carriers ( to ) enters the depletion layer under the gate. The majority of these carriers either recombines in the substrate or are directly collected by the source and drain without any probability of surmounting the Si-Si02 potential barrier. Although the last technique has been implemented in a memory array , none of the above-mentioned techniques seems to be a viable way for integration in CMOS circuits because of the danger of latchup.
0018-9383/91/0100-0111$01.00 0 1991 IEEE
IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 38, NO. 1, JANUARY 1991
,v c s
Fig. 1 . A conventional substrate hot electron injection EPROM structure. The acceleration of electrons occurs in the depletion layer (hatched) perpendicularly to the monosilicon surface.
In spite of the promising programming method for EPROM's, the SHE injection was not attractive, because it lacked an efficient source of electrons. This problem has been overcome in the so-called VIPMOS structure [ 191. The acronym VIPMOS stands for Vertical Injection Punchthrough-based MOS. This structure results in a local buried injector as the source of electrons. The basic device principle is explained in Section 11. Section I11 deals with the device fabrication. Simulations emphasize some of the advantages of this device. Furthermore, a model for implementation in a circuit simulator is presented in Section IV. Experimental results are given in Section V and Section VI summarizes the conclusions.
(b) Fig. 2. The VIPMOS structure with the local buried injector. At V, and Vd equal Vd, the punchthrough condition is not satisfied (a). Both depletion layers just touch for the case that V, and Vd equal Vdep.At a voltage V,,, punchthrough occurs and the injector emits electrons into the depletion layer underneath the gate (b).
Fig. 2 visualizes the VIPMOS structure. The VIPMOS structure has an additional n-type doped area underneath the gate. This n-type area is the buried injector and acts as the source of electrons. Apart from the injector, the structure can be similar to the conventional SHE injection EPROM, as shown in Fig. 1. In the programming mode, the injector is grounded. A high voltage VCgis applied to the control gate. Fig. 2(a) shows the VIPMOS EPROM in the case of connecting both the source and drain to a voltage Vdl.The substrate area between the MOS stack and injector is not completely depleted. Increasing the voltages on the source and drain will extend the depletion layer underneath the gate into the direction of the injector. At a certain voltage Vdep, the depletion layer will touch the depletion layer at the injector side. Further increase of the voltage leads to punchthrough (Fig. 2(b)). The punchthrough voltage VPtis defined as the voltage on the source and drain, when the injector current increases and starts to deviate from the junction saturation current. In the punchthrough mode the injector emits electrons into the depletion layer under the floating gate. These electrons will be accelerated in the electrical field. Some of them will become hot and gain sufficient energy to surmount the SiSiO, potential barrier. The injection mechanism is very efficient, because all electrons emitted by the injector are accelerated in the direction towards the Si-SiO, interface and have a chance of being collected by the floating gate. This will be illustrated in the next section. Utilization of the punchthrough mechanism for application in bipolar ROM's has already been reported by Lohstroh et al. . Mouthaan et al.  used the punchthrough mechanism in a dynamic RAM cell. In the device, presented in this paper, it is combined with the generation of hot electrons for nonvolatile memories. Actually, the local buried injector, that is activated by means of punchthrough, combines the previously described advantages of the SHE injection with an efficient source of electrons. Fig. 3 shows the energy band diagram of the VIPMOS structure under programming and read condition. The device can be characterized by two potential barriers I$,, and I$? I$f is the po-
Floating Gate SiO,
Floating Gate SiO, _.
(b) Fig. 3 . The energy band diagram of the VIPMOS structure under programming (a) and read (b) condition. The device is characterized by two potential barriers +/and +b. +/is the barrier between the injector and the substrate area above the injector, whereas +b is the Si-Si02 barrier.
WIJBURG er al.: NOVEL INJECTOR STRUCTURE FOR EPROM APPLICATIONS
tential barrier between the injector and the substrate area above the injector, whereas 4 b is the Si-Si02 potential barrier. In the programming mode, 4f is decreased when the source and drain voltage exceed Vdep.Electrons will diffuse over the lowered barrier (Fig. 3(a)) and are accelerated towards the Si-SiO, interface. Some of them may surmount the Si-SiO, barrier, the majority will be drained by either the source or drain. Fig. 3(b) shows the energy band diagram in the read mode. The injector potential is raised (e.g., it is connected to the drain voltage). Thus the barrier 4f is increased, thereby preventing the emission of electrons from the injector. In the punchthrough mode, the injector current can be written as
Active Area Definition
Field Oxide Growth
N-well Formation Overlap forms injector P-well Formation G u m e l Impl.
zinj = 1, exp with
q5f is the height of the potential barrier as indicated in Fig. 3(a)
and 4jo is the built-in potential of the junction between the injector and the substrate area above the injector. The dependence of A$ on the channel potential &h can be written as ,  A+ =
where +dep is the channel potential, when the depletion layer under the gate just touches the depletion layer at the injector side. The nonideality factor n denotes the fraction of the increasing channel Dotential that is available to forward bias the junction between the injector and the substrate area above the injector. Our devices show typical nonideality factors of 3 to 4. Using (1) and (3), the punchthrough current may be written as
In fact, the nonideality factor n is not a constant, but it gradually increases with increasing ( & h - 4 d e p ) . Assuming a highly doped injector and a homogeneously doped substrate area above the injector, a more precise expression for A+ is given by , t231
with xptis the distance from the potential minimum, when &, = q5dep, to the injector and L the distance from the Si-Si02 PI interface to the injector, as indicated in Fig. 3(a). At high currents, Zinj will become space-charge-limited and it can no longer be descnbed by an exponential behavior as in (4). For the derivation of the injector current it is assumed that the injector is grounded. For the case it is not grounded or it has a considerable resistance, &h has to be replaced by the potential difference across the punchthrough structure. Hot electron injection is often modeled by the Lucky Electron Model (LEM) -. This model was originated by Shockley  and later refined by Verwey et al. [ 111, [ 121 and Ning et al. [ 131. Following this model, the probability for an electron of being injected over the potential barrier 4b is given by pinj= A exp
Fig. 4. Process flow forming the VIPMOS structure.
where A is a fitting constant. d is the minimum distance which an electron has to travel without suffering any collisions, in order to acquire an energy equal to the Si-SO, barrier &, as indicated in Fig. 3(a). X is the scattering mean free path of an electron. Using the solution of the Poisson equation, the following expression for d can be derived, assuming a substrate area above the injector that is homogeneously doped to a concentration of N ,
where q is the electronic charge and eSiis permittivity of silicon. The height of the barrier & is affected by the electrical field in the gate oxide. Ning derived an expression for &, which incorporates the image force barrier lowering term and a “tunneling barrier lowering” term [ 131
- /3EAL2 - aE2,L3
with E,, is the electrical field in the gate oxide. a and /3 are constants. E,, is calculated by
with Vflgis the floating gate voltage, V , the flatband voltage, and T,, the gate-oxide thickness.
IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 38, NO. 1, JANUARY 1991
D I S T R X E CM1
Fig. 5 . The 1-D-doping profile of the buried injector as simulated with SUPREM 111. The solid line represents the net doping concentration, the dotted line the phosphorus concentration, and the dashed line the boron concentration.
Using the above-mentioned equations, the current flowing to the floating gate can be calculated as I"g
PI", x I,",
thereby combining the LEM with the punchthrough model.
TABLE I DIFFERENT GUMMEL A N D THRESHOLD ADJUSTMENT IMPLANTATIONS THAT HAVEBEENUSEDTO VARYTHE pWELLPROFILE, I N ORDER TO INVESTIGATEITS INFLUENCE ON THE PUNCHTHROUGH VOLTAGE, INJECTION PROBABILITY,AND NONIDEALITY FACTORn Dose (cm-2)/Energy ( k e V )
111. PROCESS DESCRIPTION AND SIMULATION The process simplicity makes the application of VIPMOS structures attractive for custom CMOS applications. The buried injector structure can easily be realized by high-energy ion implantation. In this way, the Gummel number of the substrate area above the injector can be well-controlled. This is important, because the punchthrough voltage is sensitive to the Gumme1 number. To create a local injector, the conventional buried layer does not seem to be favorable. The possible spread in the thickness and doping concentration of the epitaxial layer result in a nonreproducible Gummel number of the region above the injector. Essentially, the buried injector is formed just by an overlap of the retrograde n-well and p-well of our high-energy ion-implanted CMOS process 1251. The process flow is given in Fig. 4.The Gummel number of the substrate area above the injector is given by
Na(x)and N d ( x ) are determined by the p-well and n-well profile, respectively. The wells are implanted immediately after the field oxidation. The retrograde n-well, in which the normal PMOS devices are formed, is made by a single implantation step of 1-MeV phosphorus ions and a dose of 1 x lOI3 cm-'. The retrograde p-well is formed by a boron implantation with an energy of 350 keV and a dose of 1.5 X 10l2 cm-2. The retrograde p-well implantation determines the threshold voltage of the parasitic field-oxide NMOS. This implantation is fully covered by the overlapping n-well implantation at the injector
1.5 X 10'2/210 1.5 x 10'*/70
1.0 x 10'*/210 1.5 x 1012/70
5.0 x 10"/10 2.0 x 10"/40
5.0 x 10"/10 2.0 x 10"/40
side. An additional boron implantation with an energy of 110 keV and a dose of 1.5 x 10l2 cm-2 is done through the same mask. This implantation, further referred to as Gummel implantation, is necessary to suppress the front flank of the retrograde n-well profile. The Gummel implantation ensures a reproducible Gummel number of the substrate area above the injector. The p-well loses its retrograde character due to the Gummel implantation. The threshold voltage of the normal NMOS devices is determined by two boron implantations. The first boron implantation with an energy of 40 keV and a dose of 2 X 10" cm-2 is performed during the p-well formation. The second boron implantation, that also covers the threshold voltage adjustment of the normal PMOS devices, is a blanket implantation with an energy of 10 keV to a dose of 5 X 10" cmP2 through the gate oxide with a thickness of 25 nm. Obviously, these boron implantations also affect the Gummel number of the substrate area above the injector. The doping profile of the bur-
WIJBURG et al.: NOVEL INJECTOR STRUCTURE FOR EPROM APPLICATIONS
Fig. 6 . 2-D-doping profile of the VIPMOS structure, which is used for the device simulations.
I . 5Ee+E3 WORT = 1.5Ee+02
Fig. 7. A vector plot of the electron current density in programming mode. The dashed lines denote the junctions. The spacing between the injector and source is 5 pm. The injector is grounded V, = 5 V and Vflg = 10 V . The injection of electrons from the injector only occurs in the direction of the floating gate.
ied injector, as simulated with SUPREM 111 , is shown in Fig. 5. The junction depth, resulting from the p-well and n-well overlap (device D in Table I), is about 0.5 pm. In principle, the buried injector can be realized without any extra masking step. However, in the case of the formation of high-energy ion-implanted buried layers an n-type trunk from the buried layer up to the surface arises at the mask edge . The trunk implies an electrical connection between the buried layer and the inversion layer, preventing the VIPMOS structure from operation. In order to tackle this problem, an additional PT-masked (Preventing Trunk) implantation, 150-keV boron ions up to a dose of 5 x lo'* cm-', is carried out at the edges of the injector. Unfortunately, the PT mask increases the device dimensions at this moment. The Gummel implantation will scarcely affect the threshold voltage of the normal NMOS devices, because it is a deeper implantation. On the other hand it will considerably increase the bulk factor, especially when higher doses are used in order
to obtain a high punchthrough voltage. Also the PT implantation will have a profound effect on the bulk factor. It is interesting to investigate the influence of the Gummel number of the substrate area above the injector on the injection probability. Generally, a high Gummel number results in a high punchthrough voltage and high injection probability, whereas a lower Gummel number will give a lower punchthrough voltage and lower injection probability . In addition to the Gummel number of the region above the injector, the resulting shape of the profile of the p-well influences the injection Probability. A high boron peak near the Si-SiO? surface locally enhances the electrical field and leads to a higher injection probability. The shape of the p-well profile also influences the nonideality factor n. A deeper Gummel implantation will shift the position of the into the direction of the injector, thereby potential bamer increasing the nonideality factor n. In order to investigate these aspects, the Gummel implantation and the threshold adjustment implantations were varied. This resulted in four devices A to D
IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 38, NO. 1 , JANUARY 1991
IINJ C A) -lE-04
Fig. 8. The potential along the Si-Si02 interface at different source voltages. The source junction is situated at x = 2 pm and the injector junction at x = 7 ym. At a certain voltage, the channel potential is no longer constant along the whole injector area.
as listed in Table I. The retrograde p-well and n-well implantations were identical for all devices. Section V will deal with the measurements resulting from these devices. Fig. 6 shows the 2-D doping profile of the VIPMOS structure. This profile is used for device simulation with TRENDY, a 2-D device simulator . In the programming mode the device behavior is symmetrical. Therefore, only one half of the structure is simulated in order to save computation time. A vector plot of the electron current density under programming condition is shown in Fig. 7. The electron current density from injector towards the channel easily exceeds 200 A . cm-’ in the programming mode. The electron current density is not constant along the whole injector area. The local injector current density as well as the local injection probability is determined by the channel potential above the injector area. This channel potential itself depends on the amount of charge, which can be derived from the channel by the source and drain. This effect is emphasized in Fig. 8. It displays the channel potential along the surface from source to injector at different source voltages. Notice that at a certain source voltage, the channel potential apparently has no longer a constant value along the whole channel. This restricts the applicability of the LEM, which will be explained in the following section. As can be seen from Fig. 7, the injection of electrons occurs in vertical direction. Moreover, the injection does not occur in lateral direction, where it might trigger other structures. Holes, generated by impact ionization in the depletion layer under the floating gate, contribute to the substrate current. This substrate current may cause a parasitic bipolar action . The influence of the substrate current is suppressed by the use of a heavily doped p-type substrate . Therefore, the VIPMOS structure seems to be suitable for application in VLSI circuits without the danger of latchup. IV. VIPMOS MODEL Fig. 9 shows a typical plot of the measured injector current as a function of the draidsource to bulk voltage ( Vdsb) at different “floating” gate voltages ( Vflg).At drain/source voltages only slightly higher than the punchthrough voltage, the current has a logarithmic behavior and can be well described by (1) and (5). The injector current is independent of Vflg. The potential in the channel above the injector region is constant and fixed to a